Synthesis and characterization of core–shell gold nanoparticles with poly(vinyl pyrrolidone) from a new precursor salt
- 3.2k Downloads
In this article, we report a facile one-step chemical synthesis of gold (Au) nanoparticles (GNPs) from a new precursor salt i.e., gold hydroxide in the presence of poly(vinyl pyrrolidone) (PVP) polymer. The non-aqueous dispersion of GNPs was comprehensively characterized by UV–Visible, FTIR, zeta potential, and transmission electron microscope (TEM). A strong surface plasmon resonance band at 529 nm in the UV–Visible spectrum confirms the formation of GNPs in the Au colloid. The FTIR spectroscopic results showed that PVP molecules get chemisorbed onto the surface of GNP via O-atom of carbonyl group. A negative zeta potential of (−)16 mV reveals accumulation of nonbonding electrons of O-atom of carbonyl group of PVP molecules on the nanosurface of GNP. TEM images demonstrate a core–shell nanostructure with an Au-crystalline core covered by a thin amorphous PVP-shell. PVP-capped GNPs could be a potential candidate for bio-sensing, catalysis, and other applications.
KeywordsGold nanoparticles Core–shell nanostructure Zeta potential Chemisorption
Noble metal nanoparticles (NPs) have attracted a significant interest in materials and biological sciences owing to their potential applications in catalysis (Eustis and El-Sayed 2006; Tang et al. 2008; Daniel and Astruc 2004), biosensors (Eustis and El-Sayed 2006; Tang et al. 2008; Daniel and Astruc 2004), biomedicals (Eustis and El-Sayed 2006; Daniel and Astruc 2004; Ringe et al. 2010), photonics (Murphy et al. 2005) and heat transfer (Shalklvicht et al. 2010; Zhang et al. 2010). In recent years, gold nanoparticles (GNPs) of various sizes and shapes have received much attention from both scientists and academia because of their unique physical, chemical, photochemical, opto-electronic, and biomedical properties (Eustis and El-Sayed 2006; Tang et al. 2008; Daniel and Astruc 2004; Ringe et al. 2010; Murphy et al. 2005). The brilliant ruby color seen in stained glass windows is attributed to the presence of GNPs (Faraday 1857). Such bright color is due to collective oscillation of the electrons in the conduction band, known as surface plasmon oscillation. As the frequency of such oscillation lies in the visible region of the spectrum in gold, it gives rise to a strong surface plasmon resonance (SPR) absorption (Eustis and El-Sayed 2006; Ringe et al. 2010). Such absorption is absent in bulk metal and occurs only in nanoscale metal NPs when the incident photon frequency resonates the collective oscillation of the conduction electrons. Because of larger absorption coefficient of GNP than dye molecule, SPR is a powerful tool for biological sensors, surface-enhanced Raman spectroscopy, and many optical devices (Eustis and El-Sayed 2006; Tang et al. 2008; Daniel and Astruc 2004; Ringe et al. 2010; Murphy et al. 2005). As SPR is strongly influenced by size, shape, aggregation, composition, and the local dielectric environment of the NP (Ringe et al. 2010; Kelly et al. 2003), it can be tuned by proper selection of a synthetic route and using an efficient capping agent. Due to high surface area and surface activity, GNPs show a great tendency toward aggregation. Such agglomeration process is not required for all mentioned applications of GNPs. In this regard, a chemical method is way ahead of other synthetic routes, as it is simple, uses a weak reducing agent, and employs an efficient capping agent like poly(vinyl pyrrolidone) PVP to stop the growth process at nanoscopic level and foils aggregation of GNPs in a colloidal solution (Seo et al. 2006; Mishra et al. 2009; Ram and Fecht 2011).
Poly(vinyl pyrrolidone), an amphiphilic polymer, is a widely used encapsulating agent in the synthesis of various architectures of metal NPs (Seo et al. 2006; Mishra et al. 2009; Ram and Fecht 2011). It is not only used as a reducing/nucleating agent but also as an excellent shape and size regulating agent (Tang et al. 2008; Ringe et al. 2010; Seo et al. 2006; Mishra et al. 2009; Ram and Fecht 2011). As PVP is non-toxic and biodegradable, it possesses excellent biomedical properties (Seo et al. 2006; Mishra et al. 2009; Ram and Fecht 2011; Kamada et al. 2003) and helps in decreasing the toxicity of NPs by providing an inert coating over it. In the molecular structure of PVP, the polyvinyl backbone serves as a tail group (hydrophobic), whereas the pyrrolidone group serves as a head group (hydrophilic). The head carbonyl (C=O) groups of PVP can interact with surfaces of GNP, whereas the long tail groups can adjust the distances among adsorbed head groups to provide colloidal stability by steric effect (Seo et al. 2006; Mishra et al. 2009; Ram and Fecht 2011). Upon mesomerism in the pyrrolidone ring in the presence of a hydrogen donor (Rothschild 1972), PVP becomes reactive to build up charge-transfer complexes via O-atom with electron acceptors like fullerenes (C60/C70) (Khairullin et al. 1997 Behera and Ram 2012) and metal NPs (e.g., Au, Ag, Pt, Rh, etc.) (Seo et al. 2006; Mishra et al. 2009; Ram and Fecht 2011; Borodko et al. 2006, 2007).
In this work, a novel ultrasonic-aided one-step chemical synthesis of core–shell GNPs in the presence of PVP molecules in an alcoholic medium (i.e., in 1-butanol) was reported. Gold hydroxide Au(OH)3, a new precursor salt, tested in this work instead of widely used hydrated tetrachloro auric acid (HAuCl4·3H2O) salt for synthesis of GNPs (Tang et al. 2008; Ringe et al. 2010, Mishra et al. 2009 Ram and Fecht 2011). Samples were studied in terms of UV–Visible, Fourier transform infrared (FTIR), Zeta potential, and transmission electron microscope (TEM).
Materials and methods
Synthesis of core–shell Au-NPs
All glasswares used for the synthesis of GNPs were thoroughly cleaned in an ultrasonic bath and oven-dried prior to use. Reagent grade Au(OH)3 powder was purchased from Alfa Aesar and was dissolved in dilute HNO3 to prepare a stock solution of 0.05 M Au(NO3)3. PVP (25 kDa) and 1-butanol were purchased from Sigma Aldrich and Merck, respectively. The chemicals were used as received without further purification. At first, an alcoholic mother solution of PVP (40 g/L) was prepared in 1-butanol by mechanical stirring for 3 h at 60–70°C. After this, a specific volume of gold nitrate solution was added dropwise during stirring to a 5 mL of 40 g/L PVP solution in 1-butanol at room temperature. After magnetic stirring for 5 min, the solution was then sonicated at 50°C in an ultrasonicator (OSCAR, 20 kHz frequency and 250 W power) for 5 min so that a light purple colored nanocolloids consisting of 2 μM GNPs with 40 g/L PVP molecules were obtained in 1-butanol. Stable NF obtained was studied in terms of the UV–Visible, FTIR, Zeta potential, and microstructure.
The UV–Visible spectra of non-aqueous dispersion of GNPs with and without PVP molecules were measured under identical conditions on a Perkin Elmer double beam spectrophotometer (LAMBDA 1050) at 26°C. The sample was filled in a conventional quartz cell of 10-mm optical length and the spectra were recorded against a reference (1-butanol with 40 g/L PVP, or 1-butanol) in an identical cell. FTIR spectra were recorded on a Thermo Nicolet Corporation FTIR Spectrometer (Model NEXUS-870) in an attenuated total reflectance mode using a ZnSe crystal as a sample holder.
Zeta potential (ξ) and surface conductivity (σsc) were measured using a Malvern Nano ZS instrument using phase analysis light scattering technique. Diluted samples were sonicated for 60 s prior to measurements. Microscopic image of PVP-encapsulated Au-NPs was studied with a high resolution transmission electron microscope (HRTEM) of JEM-2100 (JEOL, Japan) operated at an accelerating voltage of 100 kV. A 50-μL colloidal gold solution was dropped on a carbon-coated 400-mesh copper grid. The grid was then dried in desiccators by keeping overnight at room temperature.
Results and discussion
UV–Visible and FTIR spectra
Zeta potential measurement
Nearly monodisperse spherical GNPs were synthesized successfully from a gold hydroxide Au(OH)3 precursor salt in the presence of PVP molecules in 1-butanol. The SPR band in UV–Visible spectrum of colloid confirms presence of GNPs in the non-aqueous system. The FTIR results indicate that PVP molecules get adsorbed on the surface of GNP via donor–acceptor type interaction between carbonyl group and GNP. A nonbonding electron transfer from O-atom of carbonyl group of PVP molecules to the surface of GNP results in a negatively charged Au surface with a zeta potential of (−)16 mV. TEM image shows formation of nearly monodisperse polymer-capped GNPs with a core–shell structure. Monodisperse PVP-capped GNPs could be a potential candidate for catalytic applications.
This work has been supported by Silicon Institute of Technology, Silicon Hills, Bhubaneswar, India.
- Ringe E, McMahon JM, Sohn K, Cobley C, Xia Y, Huang J, Schatz GC, Marks LD, Duyne RV (2010) Unravelling the effects of size, composition, and substrate on the localized surface plasmon resonance frequencies of gold and silver nanocubes: a systematic single-particle approach. J Phys Chem C 114:12511–12516CrossRefGoogle Scholar
This article is published under license to BioMed Central Ltd. Open Access This article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution and reproduction in any medium, provided the original author(s) and source are credited.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 2.0 International License (https://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.